**BEHAVIOR OF STEEL FIBRE REINFORCED **

**CONCRETE IN COMPRESSION **

R.P. Dhakal1, C. Wang1 and J.B. Mander1

1

Department of Civil Engineering, University of Canterbury, Private Bag 4800, Christchurch 8020, New Zealand

**ABSTRACT **

Standard compression tests are conducted on concrete cylinders made with concrete having different amount of steel fibres to investigate compression behaviour of steel fibre reinforced concrete. The effect of volumetric ratio of steel fibres on compressive strength, corresponding peak strain and the compressive stress-strain curve is explored. The test results show that the more the amount of fibres the higher the compressive strain the cylinder can sustain. It is also observed that both compressive strength and the strain corre sponding to the peak stress increase with the addition of steel fibres. Interrelationships relating the compressive strength and the corresponding peak strain with the volumetric ratio of steel fibres are established based on the test results. The experimental result also shows that if the compressive stress and strain are normalized with respect to the compressive strength and the peak strain respectively, the resulting normalized stress -strain curves lie close to each other and are not influenced by the fibre content. An equation to represent this unique relationship between the normalized compressive stress and strain is also proposed and verified.

**KEYWORDS **

**INTRODUCTION **

Concrete with steel fibres is proved to have better compression behaviour than plain concrete. The maximum compressive strain, which is assumed as 0.003~0.0035 for plain concrete is likely to be higher for steel fibre reinforced concrete (SFRC). Also, the post-peak softening branch of the compressive stress -strain curve of SFRC is expected to be flatter than that of plain concrete; i.e. the stress in the post-peak range is higher in SFRC. Obviously, constitutive equations representing the compressive stress-strain relationship of plain concrete cannot capture the stress -strain curves of SFRC. Not only the stress-strain curves and the equations representing thes e curves differ between SFRC and plain concrete, but they also differ between SFRC with different amount of steel fibres. Hence, generalized equations that take into account the fibre content are needed if the compressive stress and corresponding force carried by SFRC with a given fibre content are to be calculated accurately.

Test results on mortar with steel fibres have shown that the addition of fibres lead to increases in compressive strength and the strain at peak stress [Fanella and Naaman 1985]. Some studies have been done to investigate the effect of fibre content on the post-peak softening branch of the compressive stress-strain curve of SFRC [Hughes and Fattuhi 1977]. Fanella and Naaman [1985] found that an increase in the volumetric ratio of steel fibres leads to a relatively flatter post-peak softening branch in the stress-strain curve of mortar with steel fibres. Only a few attempts have been made to establish constitutive equations for SFRC [Ezeldin and Balaguru 1992], and no studies in the authors’ knowledge have led to generalized constitutive equations taking into account the fibre type and fibre content. The main objective of this paper is to investigate the compressive behaviour of SFRC with different fibre content and to explore generalized interrelationships between fibre content and the compression stress-stress curve parameters; mainly the compressive strength and the peak strain.

**EXPERIMENT DETAILS **

Standard cylinders of 100 mm diameter and 200 mm height were made of concrete with different fibre content. Six sets of twelve SFRC cylinders having 0%, 0.5%, 1.0% (two sets for two different types of fibre), 1.5% and 2.0% steel fibres (by volume) were prepared. The second and the third sets included 1.0% steel fibres of two different types commonly used in New Zealand, namely Dramix fibres [www.bekaert.com] and Novotex fibres [www.novocon.com]. This was aimed to see if the different types of steel fibres used in New Zealand had a significant effect on the compression behaviour of SFRC in general. In the other sets having 0.5%, 1.5% and 2% fibre content, Novotex fibres were used. The properties of these fibres used in the specimens are shown in Table 1.

workability of the mixes; especially the last batch with 2% steel fibres by volume was very difficult to work on.

Table 1 Steel fibre technical specification

Novotex fibre FE0730 Dramix fibre RC65/35BN

Fibre Length 30 mm 35 mm

Equivalent Diameter 0.7 mm 0.55 mm

Aspect Ratio 43 64

Tensile Strength 1150 MPa 1100 MPa

End Type Flattened ends with round shaft Hooked ends

The first batch (P1) was plain concrete without any fibres (i.e. 0% fibre content), and 12 cylinders were made from this batch. The second batch (P2) was prepared and mixed with 1% (by volume) Dramix RC65/35BN steel fibres, whereas the remaining four batches (namely P3, P2, P4, P6 and P5 respectively) were mixed with Novotex FE0730 steel fibres ranging from 0.5% to 2% by volume with an increment of 0.5%. From the five SFRC batches (P2, P3, P4, P5 and P6), six cylinders were made with the plain concrete before adding the steel fibres and the other six cylinders were made after mixing the fibres.

All cylinders were wet cured in a 200C fog room for 28 days. The cylinders were covered with plastic sheets throughout the curing period to reduce the amount of water evaporation. An AVERY 7104 DCJ Compression and Tension testing machine with a capacity of 1000 KN was used for the compression tests. The compression load was applied at a rate of 0.15 MPa per second following ASTM standard [ASTM C39/C39M -01]. In order to avoid friction that would otherwise alter the failure plane and also the measured load to some extent, a thin layer of lubricant sandwiched between two Teflon sheets was used between the loading plate and the two end surfaces of the cylinders. A high speed data logger was used to record the axial load and the corresponding deformation.

**RESULTS AND DISCUSSION **

**General Features of Compression Stress -Strain Curves **

The axial load applied to the cylinders was recorded through the actuator, and the axial deformation was measured by two potentiometers stuck on two diametrically opposite sides of each cylinder. The recorded load was divided by the initial cross-section area of the cylinders to obtain the axial compressive stress and the axial deformation was divided by the gauge length (length covered by the potentiometer) to obtain the axial compressive strain. Thus derived axial stresses for different specimens in one set are averaged and plotted against the axial strain for the six different mixes in Figure 1.

post-peak softening branch of stress-strain curves of these cylinders could not be captured. For other batches with fibre content more than 0.5%, the cylinders could be compressed without failure until the axial strain exceeded 2%, and the average stress-strain curves of these specimens clearly showed a stable post-peak softening branch. In stark contrast, the plain concrete cylinders made of the same batch of concrete before adding and mixing the fibres failed before the axial strain reached 0.5%, thereby clearly suggesting that the addition of fibres enhanced the deformability of the concrete.

**Batch P1 (No fibres) **

0 5 10 15 20 25 30 35 40 45

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

**Batch P4 (0.5% Novotex fibres)**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

Vf=0.0% Vf=0.5%

**Batch P2 (1.0% Dramix fibres)**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

Vf=0.0% Vf=1.0%

**Batch P3 (1.0% Novotex fibres)**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

Vf=0.0% Vf=1.0%

**Batch P6 1.5% Novotex fibres**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

Vf=0.0% Vf=1.5%

**Batch P5 2.0% Novotex fibres**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

[image:4.516.75.440.193.545.2]Vf=0.0% Vf=2.0%

compressive strength of the SFRC cylinders was in all batches higher than that of the plain concrete cylinders made from the same batch. The peak strain of the plain concrete in different batches varied between 0.27-0.38%; these are likely to have been overestimated as they include the strain due to the effect of creep and shrinkage. The peak strain was also found to be larger in SFRC cylinders than in plain concrete cylinders in all batches.

Table 2 Compression strength and peak strain

Series P1 P4 P2 P3 P6 P5

*Vf* (%) 0 0.5 0 1.0 0 1.0 0 1.5 0 2.0 0
Mean *f’c* 33.2 30.7 25.5 29.7 27.0 30.8 28.7 31.1 25.6 41.2 28.8
Mean *epeak* .0036 .0036 .0030 .0056 .0038 .0036 .0032 .0034 .0027 .0057 .0033

As shown in Figure 1, the stress -strain curves for the SFRC cylinders in batches P2 and P3 are noticeably different, although the corresponding curves of the plain concrete cylinders in these batches look similar except for a small difference in the compressive strength. The addition of Dramix fibres did not enhance the compressive strength but caused a significant increase in the peak strain and the rate of decrease of compressive stress in the post-peak range was smaller. On the other hand, a substantial increase in compressive strength was achieved with the addition of 1% Novotex fibres in batch 3, but the peak strain did not increase much and the rate of reduction of compressive stress in the post-peak range was higher. This indicates that Dramix fibres can sustain larger compressive strain than Novotex fibres before the stress drops to a prescribed permissible limit.

**Normalized compression stress-strain curves **

Next, the absolute values of compressive stress and strain are divided by the compressive strength and the peak strain, respectively. Figure 2 presents the average normalized compressive stress-strain curves for the P1 series (plain concrete cylinders) and other four series including the Novotex fibres (i.e. P3, P4, P5 and P6). Despite the apparently different absolute stress-strain curves in Figure 1, the normalized stress-strain curves for the different batches are very close to each other and do not indicate any correlation with the fibre content except that the normalized curves terminate early (before the normalized strain equals 2) for SFRC with fibre content less than or equal to 0.5%.

0.0 0.2 0.4 0.6 0.8 1.0 1.2

0 2 4 6 8 10

Normalized strain

Normalized stress

0%

0.5% 1.0% 1.5%

2.0% Prediction

Figure 2 Normalized compression stress -strain curves of SFRC with different fibre content

**MODELING OF COMPRESSION BEHA VIOR OF SFRC **

Earlier discussions have establis hed that the quality and amount of steel fibres affect the compressive stress -strain behaviour of concrete but the normalized stress-strain curves remain unaffected by these variables. Hence, a common equation interrelating normalized compressive stress with the normalized compressive strain is enough for SFRC with any type and quantity of fibres. Furthermore, if the average compressive strength and the peak strain of SFRC with a given quality and quantity of fibres are known, the normalized stress -strain relationship can easily be used to generate the absolute compressive stress-strain curves . As a robust mix design of SFRC is not yet available; at least not known to the authors; treating the compressive strength and peak strain of SFRC as the base variables in the model makes little sense. Nevertheless, the compressive strength and peak strain of plain concrete before adding and mixing the steel fibres can be set as the primary variables as there are well-established mix design methods to generate a given compressive strength, and the peak strain of plain concrete is a dependent variable of its compressive strength. Hence, the compressive strength and the peak strain of SFRC need to be expressed in terms of the compressive strength and peak strain of plain concrete to supplement the normalized compressive stress-strain relationship.

**Compression strength and peak strain of SFRC **

The ratio of compressive strength of the SFRC cylinders in different batches to the average
compressive strength of plain concrete cylinders made from the same batch (before adding
and mixing the steel fibres) is shown in Figure 3a. As can be seen, the compressive strength
of SFRC normalized with respect to that of plain concrete increases with an increase in fibre
content. Although there is substantial variation in the results of different specimens tested
with the same fibre content, a straight line (see Figure 3a) qualitatively represents the
dependency of the normalized compressive strength to the fibre content. The linear equation
representing this straight line, which describes the interrelationship between the volumetric
ratio of fibres (*Vf*) and the normalized compressive strength (*fpeak*/*fc’*), is given as:

*f*
*f*
*c*

*peak*

*V*
*f*

*f*

*α*

20 1

' = + (1)

where, *Vf* is the volumetric ratio of steel fibres and *αf* is an experimental constant taking into
account the quality/type of fibres. The value of *αf* is 1 for Novotex fibres and its value needs
to be calibrated before using for other types of steel fibres. For example, *αf* = 0.5 calibrates
with the results of tested SFRC cylinders with 1% Dramix fibres.

0.0 0.5 1.0 1.5 2.0

0.0 0.5 1.0 1.5 2.0 2.5

Fibre content Vf (%)

Normalized strength (f

peak

/fc

')

0.0 0.5 1.0 1.5 2.0 2.5

0.0 0.5 1.0 1.5 2.0 2.5

Fibre content Vf (%)

Normalized peak strain (e

peak

/eco

[image:7.516.76.441.318.435.2])

Figure 3 Variation of normalized compressive strength and peak strain with fibre content The ratio of peak strain of SFRC to the peak strain of plain concrete before adding and mixing the steel fibres for different specimens in different batches is plotted against the fibre content in Figure 3b. As expected, the normalized peak strain increases with an increase in fibre content. Although there is substantial scatter among the specimens having the same fibre content, a quadratic equation given in Equation 2 below qualitatively captures the increasing trend of the normalized peak strain with an increase in fibre content.

2

2000

1 *f*

*co*
*peak*

*V*
*ε*
*α*
*ε*

*ε*

+

= (2)

in which, *εco* is the peak strain of plain concrete and *αε* is an experimental constant taking
into account the quality/type of fibres. For Novotex fibres, *αε* = 1 and its value needs to be

calibrated before using for other types of steel fibres. For example, *αε* = 2.4 approximately
fits the tests results of SFRC cylinders with 1% Dramix fibres.

**Normalized compressive stress-strain relationship **

As suggested by the test results, the interrelationship between the compressive stress normalized with respect to the peak stress and the strain normalized with respect to the peak strain is independent of the fibre type and content. Of course, variation within a narrow band was observed, but the curves did not show any consistent correlation with the fibre content. Hence, only one curve passing through the centre of the narrow band can be used to represent the behaviour of SFRC with any type and amount of steel fibres. An equation to represent such a curve is given below:

2

1 _{n}_{n}

*n*
*n*

*ε*
*ε*

*ε*
*σ*

+ −

= (3)

in which, *σn* is the normalized compressive stress given by *σ */*fpeak* (where *σ* is the absolute
compressive stress and *fpeak* is the compressive strength of the SFRC to be calculated using
Equation 1, and *εn* is the normalized compressive strain given by *ε */*εpeak* (where *ε* is the
absolute compressive strain and *εpeak* is the peak strain of the SFRC to be calculated using
Equation 2). The normalized stress -strain relationship described by Equation 3, when
combined with the estimation of compressive strength (Equation 1) and peak strain
(Equation 2) of SFRC, completes the compression model of SFRC. The proposed equations
can be applied to any fibre type and content, only the constants *αf* and *αε* (in Equations 1 and
2) need to be experimentally calibrated for the fibre type.

**VERIFICATION **

The proposed model is verified by comparing with the test results. First, the normalized
compressive stress-strain relationship (Equation 3) is comp ared with the normalized average
stress-strain curves obtained from the tests for different fibre content. These curves are
plotted together with the model prediction in Figure 2. As can be seen, the model prediction
falls within the narrow band created by the experimental curves for various fibre contents.
Next in Figure 4, the absolute stress-strain curves of some cylinders with different fibre
content obtained from the tests are compared with the stress strain curves predicted by using
Equation 3 together with Equations 1 and 2. As the test results used for this comparison had
Novotex fibres, the values of *αf* and *αε* in Equations 1 and 2 are set to unity. The comparison
shows that the proposed model can fairly capture the compressive stress-strain relationship
of SFRC with different fibre content.

accurately cover the scatter of the normalized compressive strength and normalized peak strain (see Figures 3a and 3b), and hence yielded values far from those suggested by the test results of some specimens. It is found that the normalized stress-strain relationship proposed in Equation 3 did not contribute any significant proportion of the discrepancy in these specimens. Had the normalized strength and peak strain been used directly from the corresponding test results, the absolute stress-strain curves obtained by using Equation 3 would be very close to the corresponding experimental stress-strain curves.

**Batch P4 (0.5% Novotex fibres)**

0 5 10 15 20 25 30 35 40 45

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%) Stress (MPa) Prediction Specimen Specimen Specimen

**Batch P3 (1.0% Novotex fibres)**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%) Stress (MPa) Prediction Specimen Specimen

**Batch P6 (1.5% Novotex fibres)**

0 10 20 30 40

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%)

Stress (MPa)

Prediction Specimen Specimen

**Batch P5 (2.0% Novotex fibres)**

0 5 10 15 20 25 30 35 40 45

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0

Strain (%) Stress (MPa) Prediction Specimen Specimen Specimen

Figure 4 Comparison of the test results with the proposed model

It indicates that more work needs to be done; especially to establish more robust interrelationship between the normalized strength and peak strain of SFRC. More tests with different fibre content need to be conducted to get reliable data to clarify the valid range of normalized strength and peak strain, and Equations 1 and 2 could be modified accordingly, if needed. More tests are also to be conducted for different fibre types to see if the linear and quadratic assumptions of Equations 1 and 2 follow the trend in other types of steel fibres. These tests will also help to check the robustness of Equation 3.

**CONCLUSIONS**

compression tests of these SFRC cylinders, an analytical constitutive model is developed to predict the complete stress -strain curve of SFRC in monotonic compression. The following conclusions can be drawn from the outcome of this study:

1. Adding steel fibres in concrete changes the basic characteristics of its compressive stress-strain curve. The compressive strength of SFRC is higher than that of plain concrete; the peak strain is higher in SFRC than in plain concrete; SFRC can sustain larger compressive strain before crushing; and the compressive stress reduction in the post-peak softening branch of the stress-strain curve is milder in SFRC.

2. SFRC having 0.5% volumetric fibre content or less does not improve the compression deformability and will fail soon after reaching the peak, as in normal concrete. It is only for SFRC with fibre content above 0.5% that the compressive strain in excess of 2% could be applied to the cylinders before crushing.

3. The normalized compressive strength of SFRC (i.e. ratio of compression strength of SFRC to that of plain concrete) increases when volumetric fraction of steel fibres is increased, and the interrelationship can be described by a linear equation (Equation 1). 4. The normalized peak strain of SFRC (i.e. ratio of the peak strain of SFRC to that of

plain concrete) also increases when volumetric fraction of steel fibres is increased and the interrelationship can be captured by a quadratic equation (Equation 2).

5. Although Equations 1 and 2 are derived from the compression test results of SFRC
cylinders with Novotex and Dramix fibres, they can also be used for other types of steel
fibres by calibrating the experimental constants *αf* and *αε* in Equations 1 and 2,
respectively.

6. Fibre content and type affect the absolute compressive stress-strain curves of SFRC, but the normalized compressive stress-strain curves (plots of stress and strain normalized with respect to the compressive strength and peak strain respectively) lie within a narrow band regardless of the quality and quantity of steel fibres.

7. A generalized equation (Equation 3) to represent the unique normalized compressive stress-strain relationship of SFRC is proposed and verified. This equation can be used in conjunction with Equations 1 and 2 to predict the stress-strain curves of SFRC with any type and amount of steel fibres .

**REFERENCES**

1. ASTM standard (2001). *Standard Test Method for Compressive Strength of Cylindrical *

*Concrete Specimens*. ASTM C 39/C 39M -01.

2. Ezeldin A.S. and Balaguru P.N. (1992). Normal and High-Strength Fiber Reinforced
Concrete under Compression. *ASCE Journal of Materials in Civil Engineering* 4:4.
3. Fanella D.A. and Naaman A.E. (1985). Stress-Strain Properties of Fiber Reinforced

Mortar in Compression. *ACI JOURNAL* 82:4, 475-483.